electronic supplementary information rated with electronic supplementary information...
Post on 16-Jul-2020
Embed Size (px)
Electronic Supplementary Information
Plasmon-enhanced dye-sensitized solar cells using SiO2 spheres deco rated with tightly assembled silver nanoparticles
Jung-Woo Choi,1,2 Homan Kang,3 Minwoo Lee,4 Jin Soo Kang,1,2 San Kyeong,1 Jin-Kyoung Yan
g,1 Jin Kim,1,2 Dae Hong Jeong,4 Yoon-Sik Lee,1,3 and Yung-Eun Sung1,2
1 School of Chemical and Biological Engineering, Seoul National University, Seoul 151-742, Republic of Korea
2 Center for Nanoparticle Research, Institute for Basic Science (IBS), Seoul 151-742, Republic of Korea
3 Interdisciplinary Program in Nano-Science and Technology, Seoul National University, Seoul 151-742, Republic o f Korea
4 Department of Chemistry Education, Seoul National University, Seoul 137-742, Republic of Korea.
Tetraethylorthosilicate (TEOS), 3-mercaptopropyl trimethoxysilane (MPTS), ethylene glycol (E
G), poly(vinyl pyrrolidone) (PVP, MW ~40,000), silver nitrate (AgNO3, 99.99+%), octylamine (
OA), and all components of electrolyte were purchased from Sigma-Aldrich and used without fur
ther purification. Ammonium hydroxide (NH4OH, 27%) and ethanol (98%) were purchased from
Daejung Chemical. N719 (cis-diisothiocyanato-bis(2,2ʼ-bipyridyl-4,4ʼ-dicarboxylato) ruthenium(
II) bis(tetrabutylammonium)) dye was purchased from Solaronix.
2. Preparation of SiO2 spheres decorated with tightly assembled silver nanoparticles
Tetraethylorthosilicate (TEOS, 1.6 mL) was dissolved in 40 mL of absolute ethanol, followed b
y addition of a 3 mL portion of aqueous ammonium hydroxide (27%). The resulting mixture was
vigorously stirred using magnetic bar for 20 h at 25 °C. The resulting silica spheres were centrifu
Electronic Supplementary Material (ESI) for RSC Advances. This journal is © The Royal Society of Chemistry 2014
ged and then washed with ethanol five times to remove the excess reagents. These silica spheres
were then functionalized with thiol group. Silica spheres (150 mg) were dispersed in 3 mL ethan
ol containing 150 μL of MPTS and 30 μL of aqueous ammonium hydroxide (27 %). The mixture
was stirred for 12 h at 25 °C. The resulting MPTS-treated silica spheres were centrifuged and wa
shed with ethanol several times. In order to fabricate SiO2 spheres decorated with tightly assembl
ed silver nanoparticles (SiO2-t-Ag), 25 mg portion of MPTS-treated silica spheres was thoroughl
y dispersed in 100 mL of AgNO3 solution (3.5 mM in ethylene glycol). An 82.7 µL of octylamin
e (5 mM) was then rapidly added into the MPTS-treated silica spheres dispersion. The resulting
mixture was stirred for 1 h at 25 °C. Afterwards, SiO2 spheres decorated with tightly assembled s
ilver nanoparticles were centrifuged and washed with ethanol five times for purification. In case
of SiO2 spheres decorated with sparsely assembled silver nanoparticles (SiO2-s-Ag), 50 mg of M
PTS-treated silica spheres was used in the same reaction condition except amount of SiO2 sphere.
For silica coating to SiO2 spheres decorated with tightly assembled silver nanoparticles, a 1 mL
portion of MPTS solution (2 mM in ethanol) was added into 1 mg of silver nanoparticles-decorat
ed silica spheres. The resulting dispersion was shaken for 1 h at 25 °C. The silver nanoparticles-d
ecorated silica spheres were transferred to 50 mL of 2-propanol with 1 mg of PVP (MW ~40,000
). A 2 ml of ammonium hydroxide was added to the reaction mixture under vigorous stirring, foll
owed by the addition of 250 μL of TEOS solution (TEOS/2-propanol, 0.8 v/v %) in two separate
portions with a time interval of 30 min. After adding the TEOS, the mixture was allowed to react
for 12 h. Finally, the resulting silica coated SiO2 spheres decorated with tightly assembled silver
nanoparticles (SiO2-t-Ag@SiO2) were centrifuged and washed with ethanol five times.
3. Preparation of the photoanodes
F-doped SnO2 (FTO) glass plates (8 Ω/cm2, Pilkington TEC glassTM) were cleaned in detergent s
olution using an ultrasonic bath for 20 min and washed with tap water and ethanol. The plates we
re immersed in 40 mM TiCl4 aqueous solution at 70 °C for 30 min and rinsed with DI water and
ethanol. The photoanode pastes incorporating SiO2-t-Ag@SiO2 or SiO2 were prepared by simple
mixing. The SiO2-t-Ag@SiO2 or SiO2 in ethanol solutions (SiO2 to TiO2 ratio = 1, 3 wt%) were
mixed with commercial TiO2 pastes (Dyesol, DSL 18NR-T), and they were stirred for 2 h and di
spersed by ultrasonicator. Then ethanol was removed by rotary evaporator. The photoanode films
were prepared by Doctor blade printing on TiCl4-treated FTO plates, and annealed at 500 °C for
15 min. The thickness and the active area of photoanode films were controlled to 6 μm and 0.202
4. Assembly of dye-sensitized solar cells
Cathodes were prepared by thermal deposition. A drop of 10 mM H2PtCl6 in 2-propanol was spr
ead on FTO glass plate by spin coating followed by heating to 400 °C for 15 min. The prepared p
hotoanode was assembled with Pt counter electrode (with drilled hole) into sandwich-type cell us
ing thermal adhesive film (Surlyn: 30 μm, Dupont). The electrolyte solution was prepared by mix
ing 0.60 M 1-butyl-3-methylimidazolium iodide, 0.03 M I2, 0.10 M guanidinium thiocyanate and
4-tert-butylpyridine in a mixture of acetonitrile and valeronitrile (v/v, 85:15). Before the measure
ment of photovoltaic performance, a mask of 0.16 cm2 was attached on the outside of FTO glass
having the photoanode.
UV-Vis absorption spectra of the particles in solutions were collected by a UV-Visible spectro
meter (Mecasys Co. Ltd., Optizen 2120 UV). UV-vis absorption and reflectance spectra of the ph
otoanodes were collected by UV-vis spectrometer (Jasco, V-670) with integrated sphere. A TE
M images were obtained using EF-TEM (Carl Zeiss, LIBRA 120). The photovoltaic performance
was measured using a 500 W xenon lamp (XIL model 05A50KS source measure units and an A
M 1.5 filter) at a power of 100 mW/cm2. The incident photon-to-current efficiency was measured
using solar cell quantum efficiency measurement system (QEX10, PV measurements, Inc.).
6. Individual silver nanoparticles and SiO2 spheres decorated with sparsely assembled silve
r nanoparticles (SiO2-s-Ag)
Fig. S1 TEM image of (a) individual Ag NPs and (b) SiO2 spheres decorated with sparsely assembled silver nanopar ticles (SiO2-s-Ag).
Fig. S2 UV-vis absorption spectra of SiO2 spheres decorated with sparsely assembled silver nanoparticles (SiO2-s-A g) and SiO2 spheres decorated with tightly assembled silver nanoparticles (SiO2-t-Ag).
7. UV-vis absorption and diffused reflectance spectra of photoanodes before dye-adsorption
Fig. S3 (a) UV-vis absorption spectra of photoanodes before dye-adsorption (b) UV-vis diffused reflectance spectra of photoanodes before dye-adsorption.
8. Optical and photoelectrochemical properties of 5 wt% SiO2-t-Ag@SiO2 photoanode cell
To obtain an optimized performance, paste containing 5 wt% of SiO2-t-Ag@SiO2 was prepared.
The photoanode containing 5 wt% of SiO2-t-Ag@SiO2 shows stronger UV-vis absorption becaus
e of higher concentration of SiO2-t-Ag@SiO2. (Fig. S4(a)) However, It exhibit lower photo-curre
nt and power conversion efficiency than 3 wt% cell. (Fig. S4(b,c)) It is mainly due to excessive li
ght absorption by SiO2-t-Ag@SiO2, which isn`t delivered to the sensitizer completely.
Fig. S4 (a) UV-vis absorption spectra of photoanodes, (b) J-V curves of DSSCs, (c) IPCE spectra of DSSCs.
9. Discrete Dipole Approximation (DDA) simulations
To further study the origin of the increased short-circuit current, we simulated the electric filed
distribution around the light-illuminated SiO2 sphere decorated with silver nanoparticles by using
the DDSCAT 7.1 package . In our simulation, isotropic dipoles are evenly placed in silver nan
oparticles at dipole–dipole distances of 2 nm. These silver nanoparticles were 20 nm in diameter,
and the distance between each silver nanoparticle is about 2 nm, and silica core was 160 nm in di
ameter. From this DDA simulation results, a strong electric field at the surface of silver was obse
rved. Also, the enhanced field was confirmed outside of the SiO2 shell. The enhanced electric fiel
d around silver nanoparticle increases the absorption of N719 dye adsorbed on adjacent TiO2.
Fig. S5 (a) Electric field intensity distribution in SiO2 sphere decorated with silver nanoparticles, (b) showing a clos e up silver nanoparticle surface, (c) Intensity of electric fields with respect to the distance from silver nanoparticle.
10. Photovoltaic characteristics of DSSCs with 12 μm photoanodes (TiO2 and 3 wt% SiO2-t-
Fig. S6 J-V curves of DSSCs with 12 μm photoanodes.
Table S1 Photovoltaic parameters of DSSCs with 12 μm photoanodes
Photoanode JSC (mA/cm2) VOC (V) ff η (%)
TiO2 (12 μm) 14.84 0.703 0.71 7.44
3 wt% SiO2-t-Ag@SiO2 (12 μm) 16.18 0.731 0.70 8.31
11. Absorbed photon-to-current conversion efficiency (APCE)
The absorbed photon-to-current conversion efficiency (APCE) was calculated by dividing